#------------------------------------------------------------------------------
#$Date: 2016-03-21 01:21:50 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178377 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/07/4000797.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000797
loop_
_publ_author_name
'Meng, Chang-Yu'
'Chen, Hong'
'Wang, Peng'
'Chen, Ling'
_publ_section_title
;
 Syntheses, Structures, and Magnetic and Thermoelectric Properties of
 Double-Tunnel Tellurides: AxRE2Cu6--xTe6(A = K--Cs; RE = La--Nd)
;
_journal_issue                   22
_journal_name_full               'Chemistry of Materials'
_journal_page_first              4910
_journal_paper_doi               10.1021/cm201574a
_journal_volume                  23
_journal_year                    2011
_chemical_formula_moiety         'Cu1.76 La0.67 Rb0.24 Te2'
_chemical_formula_sum            'Cu1.76 La0.67 Rb0.24 Te2'
_chemical_formula_weight         480.15
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   10.0056(8)
_cell_length_b                   10.0056(8)
_cell_length_c                   4.2336(6)
_cell_measurement_reflns_used    456
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.3794
_cell_measurement_theta_min      2.3503
_cell_volume                     367.05(7)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2007)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 13.6612
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  SCXMini
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0302
_diffrn_reflns_av_sigmaI/netI    0.0156
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            2858
_diffrn_reflns_theta_full        27.38
_diffrn_reflns_theta_max         27.38
_diffrn_reflns_theta_min         2.35
_exptl_absorpt_coefficient_mu    27.196
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.5773
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            gray
_exptl_crystal_density_diffrn    6.517
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             606
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.11
_refine_diff_density_max         1.863
_refine_diff_density_min         -1.186
_refine_diff_density_rms         0.218
_refine_ls_extinction_coef       0.0046(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.244
_refine_ls_matrix_type           full
_refine_ls_number_parameters     23
_refine_ls_number_reflns         316
_refine_ls_number_restraints     14
_refine_ls_restrained_S_all      1.358
_refine_ls_R_factor_all          0.0240
_refine_ls_R_factor_gt           0.0231
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0184P)²+2.6063P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0498
_refine_ls_wR_factor_ref         0.0503
_reflns_number_gt                309
_reflns_number_total             316
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm201574a_si_001.cif
_cod_data_source_block           Rb0.72La2Cu5.29Te6
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      P6(3)/m
_cod_database_code               4000797
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Rb1 Rb 0.0000 0.0000 0.2500 0.058(5) Uani 0.196(12) 6 d SPU
Rb2 Rb 0.0000 0.0000 0.0000 0.056(6) Uani 0.162(12) 6 d SPU
La La 0.6667 0.3333 0.2500 0.0157(3) Uani 1 6 d S
Cu Cu 0.03535(14) 0.43285(15) 0.2500 0.0201(3) Uani 0.881(3) 2 d SPU
Te Te 0.27411(6) 0.38927(6) 0.2500 0.0160(2) Uani 1 2 d SU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Rb2 Rb1 Rb2 180.0 4 .
Rb2 Rb1 Rb1 0.0 4 7_556
Rb2 Rb1 Rb1 180.0 . 7_556
Rb2 Rb1 Rb1 180.0 4 7
Rb2 Rb1 Rb1 0.0 . 7
Rb1 Rb1 Rb1 180.0 7_556 7
Rb2 Rb1 Rb2 180.0 4 4_554
Rb2 Rb1 Rb2 0.0 . 4_554
Rb1 Rb1 Rb2 180.0 7_556 4_554
Rb1 Rb1 Rb2 0.0 7 4_554
Rb2 Rb1 Rb2 0.0 4 1_556
Rb2 Rb1 Rb2 180.0 . 1_556
Rb1 Rb1 Rb2 0.0 7_556 1_556
Rb1 Rb1 Rb2 180.0 7 1_556
Rb2 Rb1 Rb2 180.0 4_554 1_556
Rb2 Rb1 Te 90.0 4 .
Rb2 Rb1 Te 90.0 . .
Rb1 Rb1 Te 90.0 7_556 .
Rb1 Rb1 Te 90.0 7 .
Rb2 Rb1 Te 90.0 4_554 .
Rb2 Rb1 Te 90.0 1_556 .
Rb2 Rb1 Te 90.0 4 2
Rb2 Rb1 Te 90.0 . 2
Rb1 Rb1 Te 90.0 7_556 2
Rb1 Rb1 Te 90.0 7 2
Rb2 Rb1 Te 90.0 4_554 2
Rb2 Rb1 Te 90.0 1_556 2
Te Rb1 Te 120.0 . 2
Rb2 Rb1 Te 90.0 4 3
Rb2 Rb1 Te 90.0 . 3
Rb1 Rb1 Te 90.0 7_556 3
Rb1 Rb1 Te 90.0 7 3
Rb2 Rb1 Te 90.0 4_554 3
Rb2 Rb1 Te 90.0 1_556 3
Te Rb1 Te 120.0 . 3
Te Rb1 Te 120.0 2 3
Rb2 Rb1 Te 121.417(6) 4 7
Rb2 Rb1 Te 58.583(6) . 7
Rb1 Rb1 Te 121.417(6) 7_556 7
Rb1 Rb1 Te 58.583(6) 7 7
Rb2 Rb1 Te 58.583(6) 4_554 7
Rb2 Rb1 Te 121.417(6) 1_556 7
Te Rb1 Te 148.583(6) . 7
Te Rb1 Te 64.742(2) 2 7
Te Rb1 Te 64.742(2) 3 7
Rb2 Rb1 Te 58.583(6) 4 8_556
Rb2 Rb1 Te 121.417(6) . 8_556
Rb1 Rb1 Te 58.583(6) 7_556 8_556
Rb1 Rb1 Te 121.417(6) 7 8_556
Rb2 Rb1 Te 121.417(6) 4_554 8_556
Rb2 Rb1 Te 58.583(6) 1_556 8_556
Te Rb1 Te 64.742(2) . 8_556
Te Rb1 Te 148.583(6) 2 8_556
Te Rb1 Te 64.742(2) 3 8_556
Te Rb1 Te 129.484(3) 7 8_556
Rb2 Rb1 Te 58.583(6) 4 9_556
Rb2 Rb1 Te 121.417(6) . 9_556
Rb1 Rb1 Te 58.583(6) 7_556 9_556
Rb1 Rb1 Te 121.417(6) 7 9_556
Rb2 Rb1 Te 121.417(6) 4_554 9_556
Rb2 Rb1 Te 58.583(6) 1_556 9_556
Te Rb1 Te 64.742(2) . 9_556
Te Rb1 Te 64.742(2) 2 9_556
Te Rb1 Te 148.583(6) 3 9_556
Te Rb1 Te 129.484(3) 7 9_556
Te Rb1 Te 95.303(8) 8_556 9_556
Rb1 Rb2 Rb1 180.0 7 .
Rb1 Rb2 Rb2 180.0 7 4
Rb1 Rb2 Rb2 0.0 . 4
Rb1 Rb2 Rb2 0.0 7 4_554
Rb1 Rb2 Rb2 180.0 . 4_554
Rb2 Rb2 Rb2 180.0 4 4_554
Rb1 Rb2 Rb1 0.0 7 1_554
Rb1 Rb2 Rb1 180.0 . 1_554
Rb2 Rb2 Rb1 180.0 4 1_554
Rb2 Rb2 Rb1 0.0 4_554 1_554
Rb1 Rb2 Rb1 180.0 7 7_556
Rb1 Rb2 Rb1 0.0 . 7_556
Rb2 Rb2 Rb1 0.0 4 7_556
Rb2 Rb2 Rb1 180.0 4_554 7_556
Rb1 Rb2 Rb1 180.0 1_554 7_556
Rb1 Rb2 Te 106.983(4) 7 .
Rb1 Rb2 Te 73.017(4) . .
Rb2 Rb2 Te 73.017(4) 4 .
Rb2 Rb2 Te 106.983(4) 4_554 .
Rb1 Rb2 Te 106.983(4) 1_554 .
Rb1 Rb2 Te 73.017(4) 7_556 .
Rb1 Rb2 Te 73.017(4) 7 7
Rb1 Rb2 Te 106.983(4) . 7
Rb2 Rb2 Te 106.983(4) 4 7
Rb2 Rb2 Te 73.017(4) 4_554 7
Rb1 Rb2 Te 73.017(4) 1_554 7
Rb1 Rb2 Te 106.983(4) 7_556 7
Te Rb2 Te 180.000(15) . 7
Rb1 Rb2 Te 73.017(4) 7 8
Rb1 Rb2 Te 106.983(4) . 8
Rb2 Rb2 Te 106.983(4) 4 8
Rb2 Rb2 Te 73.017(4) 4_554 8
Rb1 Rb2 Te 73.017(4) 1_554 8
Rb1 Rb2 Te 106.983(4) 7_556 8
Te Rb2 Te 68.159(3) . 8
Te Rb2 Te 111.841(3) 7 8
Rb1 Rb2 Te 106.983(4) 7 2
Rb1 Rb2 Te 73.017(4) . 2
Rb2 Rb2 Te 73.017(4) 4 2
Rb2 Rb2 Te 106.983(4) 4_554 2
Rb1 Rb2 Te 106.983(4) 1_554 2
Rb1 Rb2 Te 73.017(4) 7_556 2
Te Rb2 Te 111.841(3) . 2
Te Rb2 Te 68.159(3) 7 2
Te Rb2 Te 180.0 8 2
Rb1 Rb2 Te 73.017(4) 7 9
Rb1 Rb2 Te 106.983(4) . 9
Rb2 Rb2 Te 106.983(4) 4 9
Rb2 Rb2 Te 73.017(4) 4_554 9
Rb1 Rb2 Te 73.017(4) 1_554 9
Rb1 Rb2 Te 106.983(4) 7_556 9
Te Rb2 Te 68.159(3) . 9
Te Rb2 Te 111.841(3) 7 9
Te Rb2 Te 111.841(3) 8 9
Te Rb2 Te 68.159(3) 2 9
Rb1 Rb2 Te 106.983(4) 7 3
Rb1 Rb2 Te 73.017(4) . 3
Rb2 Rb2 Te 73.017(4) 4 3
Rb2 Rb2 Te 106.983(4) 4_554 3
Rb1 Rb2 Te 106.983(4) 1_554 3
Rb1 Rb2 Te 73.017(4) 7_556 3
Te Rb2 Te 111.841(3) . 3
Te Rb2 Te 68.159(3) 7 3
Te Rb2 Te 68.159(3) 8 3
Te Rb2 Te 111.841(3) 2 3
Te Rb2 Te 180.000(14) 9 3
Te La Te 79.798(15) 9_656 9_655
Te La Te 134.888(5) 9_656 8
Te La Te 83.272(11) 9_655 8
Te La Te 83.272(11) 9_656 8_556
Te La Te 134.888(5) 9_655 8_556
Te La Te 79.798(15) 8 8_556
Te La Te 83.272(11) 9_656 7_666
Te La Te 134.888(5) 9_655 7_666
Te La Te 134.888(5) 8 7_666
Te La Te 83.272(11) 8_556 7_666
Te La Te 134.888(5) 9_656 7_665
Te La Te 83.272(11) 9_655 7_665
Te La Te 83.272(11) 8 7_665
Te La Te 134.888(5) 8_556 7_665
Te La Te 79.798(15) 7_666 7_665
Te La Cu 46.790(14) 9_656 1_655
Te La Cu 46.790(14) 9_655 1_655
Te La Cu 129.946(15) 8 1_655
Te La Cu 129.946(15) 8_556 1_655
Te La Cu 92.44(2) 7_666 1_655
Te La Cu 92.44(2) 7_665 1_655
Te La Cu 92.44(2) 9_656 3
Te La Cu 92.44(2) 9_655 3
Te La Cu 46.790(14) 8 3
Te La Cu 46.790(14) 8_556 3
Te La Cu 129.946(15) 7_666 3
Te La Cu 129.946(15) 7_665 3
Cu La Cu 120.0 1_655 3
Te La Cu 129.946(15) 9_656 2_665
Te La Cu 129.946(15) 9_655 2_665
Te La Cu 92.44(2) 8 2_665
Te La Cu 92.44(2) 8_556 2_665
Te La Cu 46.790(14) 7_666 2_665
Te La Cu 46.790(14) 7_665 2_665
Cu La Cu 120.0 1_655 2_665
Cu La Cu 120.0 3 2_665
Te La Cu 95.31(2) 9_656 9_655
Te La Cu 45.91(2) 9_655 9_655
Te La Cu 45.75(2) 8 9_655
Te La Cu 95.19(2) 8_556 9_655
Te La Cu 178.011(14) 7_666 9_655
Te La Cu 102.189(17) 7_665 9_655
Cu La Cu 87.58(4) 1_655 9_655
Cu La Cu 48.61(3) 3 9_655
Cu La Cu 134.70(3) 2_665 9_655
Te La Cu 45.91(2) 9_656 9_656
Te La Cu 95.31(2) 9_655 9_656
Te La Cu 95.19(2) 8 9_656
Te La Cu 45.75(2) 8_556 9_656
Te La Cu 102.189(17) 7_666 9_656
Te La Cu 178.011(14) 7_665 9_656
Cu La Cu 87.58(4) 1_655 9_656
Cu La Cu 48.61(3) 3 9_656
Cu La Cu 134.70(3) 2_665 9_656
Cu La Cu 75.82(3) 9_655 9_656
Te La Cu 45.75(2) 9_656 7_666
Te La Cu 95.19(2) 9_655 7_666
Te La Cu 178.011(14) 8 7_666
Te La Cu 102.189(17) 8_556 7_666
Te La Cu 45.91(2) 7_666 7_666
Te La Cu 95.31(2) 7_665 7_666
Cu La Cu 48.61(3) 1_655 7_666
Cu La Cu 134.70(3) 3 7_666
Cu La Cu 87.58(4) 2_665 7_666
Cu La Cu 133.533(9) 9_655 7_666
Cu La Cu 86.198(19) 9_656 7_666
Te Cu Te 107.62(5) 9 9_556
Te Cu Te 115.99(3) 9 3_565
Te Cu Te 115.99(3) 9_556 3_565
Te Cu Te 101.15(4) 9 .
Te Cu Te 101.15(4) 9_556 .
Te Cu Te 112.97(5) 3_565 .
Te Cu Cu 134.35(7) 9 7_566
Te Cu Cu 58.04(3) 9_556 7_566
Te Cu Cu 57.95(5) 3_565 7_566
Te Cu Cu 123.41(5) . 7_566
Te Cu Cu 58.04(3) 9 7_565
Te Cu Cu 134.35(7) 9_556 7_565
Te Cu Cu 57.95(5) 3_565 7_565
Te Cu Cu 123.41(5) . 7_565
Cu Cu Cu 99.11(8) 7_566 7_565
Te Cu La 66.50(3) 9 1_455
Te Cu La 66.50(3) 9_556 1_455
Te Cu La 90.40(4) 3_565 1_455
Te Cu La 156.64(5) . 1_455
Cu Cu La 68.31(5) 7_566 1_455
Cu Cu La 68.31(5) 7_565 1_455
Te Cu La 161.27(4) 9 7_666
Te Cu La 87.435(16) 9_556 7_666
Te Cu La 64.21(2) 3_565 7_666
Te Cu La 64.14(2) . 7_666
Cu Cu La 63.07(4) 7_566 7_666
Cu Cu La 118.84(6) 7_565 7_666
La Cu La 131.39(3) 1_455 7_666
Te Cu La 87.435(16) 9 7_665
Te Cu La 161.27(4) 9_556 7_665
Te Cu La 64.21(2) 3_565 7_665
Te Cu La 64.14(2) . 7_665
Cu Cu La 118.84(6) 7_566 7_665
Cu Cu La 63.07(4) 7_565 7_665
La Cu La 131.39(3) 1_455 7_665
La Cu La 75.82(3) 7_666 7_665
Te Cu Rb1 69.26(3) 9 .
Te Cu Rb1 69.26(3) 9_556 .
Te Cu Rb1 168.94(5) 3_565 .
Te Cu Rb1 55.98(3) . .
Cu Cu Rb1 126.33(5) 7_566 .
Cu Cu Rb1 126.33(5) 7_565 .
La Cu Rb1 100.66(3) 1_455 .
La Cu Rb1 107.51(3) 7_666 .
La Cu Rb1 107.51(3) 7_665 .
Cu Te Cu 107.62(5) 8_556 8
Cu Te Cu 64.01(3) 8_556 2_665
Cu Te Cu 64.01(3) 8 2_665
Cu Te Cu 125.44(2) 8_556 .
Cu Te Cu 125.44(2) 8 .
Cu Te Cu 127.03(5) 2_665 .
Cu Te La 66.71(3) 8_556 7_666
Cu Te La 129.79(4) 8 7_666
Cu Te La 70.04(2) 2_665 7_666
Cu Te La 69.95(2) . 7_666
Cu Te La 129.79(4) 8_556 7_665
Cu Te La 66.71(3) 8 7_665
Cu Te La 70.04(2) 2_665 7_665
Cu Te La 69.95(2) . 7_665
La Te La 79.798(15) 7_666 7_665
Cu Te Rb1 99.31(3) 8_556 .
Cu Te Rb1 99.31(3) 8 .
Cu Te Rb1 147.99(3) 2_665 .
Cu Te Rb1 84.98(3) . .
La Te Rb1 130.816(11) 7_666 .
La Te Rb1 130.816(11) 7_665 .
Cu Te Rb2 112.98(3) 8_556 .
Cu Te Rb2 85.36(3) 8 .
Cu Te Rb2 144.19(3) 2_665 .
Cu Te Rb2 85.20(3) . .
La Te Rb2 144.339(14) 7_666 .
La Te Rb2 115.962(10) 7_665 .
Rb1 Te Rb2 16.983(4) . .
Cu Te Rb2 85.36(3) 8_556 4
Cu Te Rb2 112.98(3) 8 4
Cu Te Rb2 144.19(3) 2_665 4
Cu Te Rb2 85.20(3) . 4
La Te Rb2 115.962(10) 7_666 4
La Te Rb2 144.339(14) 7_665 4
Rb1 Te Rb2 16.983(4) . 4
Rb2 Te Rb2 33.966(7) . 4
Cu Te Rb1 123.97(3) 8_556 7
Cu Te Rb1 73.58(3) 8 7
Cu Te Rb1 136.36(2) 2_665 7
Cu Te Rb1 85.71(3) . 7
La Te Rb1 153.146(16) 7_666 7
La Te Rb1 102.912(10) 7_665 7
Rb1 Te Rb1 31.417(6) . 7
Rb2 Te Rb1 14.434(2) . 7
Rb2 Te Rb1 48.400(10) 4 7
Cu Te Rb1 73.58(3) 8_556 7_556
Cu Te Rb1 123.97(3) 8 7_556
Cu Te Rb1 136.36(2) 2_665 7_556
Cu Te Rb1 85.71(3) . 7_556
La Te Rb1 102.912(9) 7_666 7_556
La Te Rb1 153.146(16) 7_665 7_556
Rb1 Te Rb1 31.417(6) . 7_556
Rb2 Te Rb1 48.400(10) . 7_556
Rb2 Te Rb1 14.434(2) 4 7_556
Rb1 Te Rb1 62.834(12) 7 7_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La Te 3.3001(5) 9_656
La Te 3.3001(5) 9_655
La Te 3.3001(5) 8
La Te 3.3001(5) 8_556
La Te 3.3001(5) 7_666
La Te 3.3001(5) 7_665
La Cu 3.3055(13) 1_655
La Cu 3.3055(13) 3
La Cu 3.3055(13) 2_665
La Cu 3.4451(10) 9_655
La Cu 3.4451(10) 9_656
La Cu 3.4451(10) 7_666
Cu Te 2.6229(8) 9
Cu Te 2.6229(8) 9_556
Cu Te 2.6255(14) 3_565
Cu Te 2.6342(14) .
Cu Cu 2.7816(17) 7_566
Cu Cu 2.7816(17) 7_565
Cu La 3.3055(13) 1_455
Cu La 3.4451(10) 7_666
Cu La 3.4451(10) 7_665
Te Cu 2.6229(8) 8_556
Te Cu 2.6229(8) 8
Te Cu 2.6255(14) 2_665
Te La 3.3001(5) 7_666
Te La 3.3001(5) 7_665
